PART III –
Maintenance and repair
What to look for and how to take care of your FRP boat
For everyday use, fibreglass reinforced polyester generally does not need much maintenance but this does not mean the boat will last forever. Wear and tear and the absorption of water do affect the lifespan of an FRP boat. The challenge is to determine if what can be observed on the surface is just cosmetic or more serious structural damage.
If unattended for a long time, a good quality FRP boat has the advantage of not requiring as much maintenance as a wooden boat.
A boat’s smooth shiny surfaces can be protected by a good polishing with wax. This polish repels water and helps to keep the surface clean. Polishing is not a realistic option for rough surfaces like the inside surface of a boat. Wear and tear is often heaviest in these areas where the only protection is a layer topcoat.
FRP is brittle compared to wood, and is fairly easily damaged when dragged over or hitting rocks!
Check the boat for cracks after hitting hard objects and repair as soon as possible!
Do not use a bigger engine than the boat is intended for!
It is important to watch out for new cuts and crushing on the surface. Any such areas should be examined and sealed temporarily especially if the cracks are deep. As soon as possible, the damage should be repaired properly to prevent the areas from developing into more severe structural damage as a result of material fatigue during continued use of the boat.
When the surface becomes too worn, it should be degreased, cleaned and abraded properly to give good adhesion for a fresh layer of topcoat or paint. Above the waterline, a good quality marine paint is often a quicker, short-term solution than applying new topcoat. Paint has a glossier surface, and more easily repels dirt. However, gelcoat builds up thicker and generally resists mechanical wear better.
When a boat is left in the water constantly, water is absorbed by the polyester laminate. Gelcoat or topcoat does not stop water absorption. This absorption is not visible, but the laminate can absorb 1.5 to 2 percent water and become less stiff. After some years (5 to 15) the laminate can also react chemically with the water to produce hydrolysation which is comparable to rust in steel. The speed and extent of hydrolysation depends on the combination of water conditions, temperature, use of the boat, and how good the quality control was when the boat was built.
In this picture, old laminate showing typical results of hydrolysation can be seen. The polyester becomes depolymerized and is washed out of the laminate.
The results are visible as dark spots on the surface and white pockets deeper in the laminate. If the gelcoat is intact, osmosis blisters might occur.
Old laminate is weaker and less stiff than new laminate, even if damage is not visible.
This photo shows typically worn interior of a fishing boat. The topcoat is worn off, and even FRP laminate covering the longitudinal stiffeners is gone. The damaged laminate should already have been repaired to regain original strength and the surface recoated with topcoat or paint.
Water absorption will be slowed and working life of the boat improved if the hull laminate below the waterline is treated with several layers of epoxy barrier coat when the boat is new. Anti-fouling material applied to the hull to reduce marine growth improves fuel economy but has no effect on water absorption.
FIGURE 91 FIGURE 90
This photo shows what happens when laminate has not been maintained or repaired for too long.
The laminate has lost its strength and stiffness and, due to fatigue, the frame has broken.
At this spot the longitudinal stiffener is no longer supported by FRP laminate and, as a result, the bottom laminate can flex.
For fishing boats and workboats making and maintaining a glossy surface finish is not always realistic. However, such surfaces repel water more easily and take longer to deteriorate.
The goal of regular maintenance is to keep the vessel in a state of good repair and help it last as long as possible. The next two chapters focus on how to repair a damaged boat so that it is sound and as close to the original in strength and stiffness as possible. If such action is needed suggestions for improving the boat, compared to the original, are also given.
REPAIRING SMALL DEFECTS
The following notes refer to the repair of minor damage to FRP boats where the gelcoat has worn away or been chipped or cut but the laminate has not been seriously abraded. Figures 91 to 93 show an example of superficial damage and the steps needed in preparation for making the repair.
First of all, make sure it is really just a minor defect.
If the laminate is damaged, the site needs structural repair (as described in the section titled “Repairing structural damage”).
Dirt, oil from the engine, grease, and blood from fish must be cleaned off before sanding begins!
Soap and water are used first followed by washing with available strong detergent.
All broken gelcoat must be sanded away and any broken edges like the ones shown in Figure 91 must be smoothed.
A small piece of sandpaper (60 to 100 grit) should be used and size of repair area kept to a minimum.
Once sanded, no further washing or degreasing should occur before applying topcoat to the damaged area!
Topcoat should be prepared be combining the following ingredients in the proportions shown (half a litre of gelcoat, 20 ml of wax and 10 ml of MEK peroxide).
Figures 94 to 96 were copied from a repair folder. In Figure 94, the formula for topcoat is shown graphically. Figure 95 explains the two measures used in the above formula where a plastic bottle is cut down to hold half a litre (500 ml) and each bottle cap holds 5 ml (see Figure 95). Such measuring devices are readily available and provide a simple way to get the right ratio of materials for a good cure.
If there is a very thick layer of gelcoat and/or the damage extends slightly into the laminate but is not deep enough to be considered structural damage, the area can be repaired faster using putty. To make putty, mix in Colloidal Silica, the preferred option, or Talcome, if this is what is available, according to the formula in Figure 96. The amount of talcome/silica required depends on how much is needed to achieve the viscosity suitable for repairing the damaged area.
It needs to be emphasized that putty is much weaker than laminate and is not a good structural substitute for fibreglass reinforced polyester!
To create a lasting finish on the surface, the putty should be sanded down and a layer of topcoat added. At this stage, the appearance of the cured topcoat will be slightly rough and dull. To get a smooth and shiny finish, it is necessary to water sand the topcoat with an 800 grit (or finer). This should be followed by buffing and polishing to the same standard used for making plugs or repairing moulds.
REPAIRING STRUCTURAL DAMAGE
Practical guidelines for structural FRP repair
In general, repairing FRP boats can be easier than repairs involving other materials. However, proper preparation of the site, a dry working environment and the correct air temperature are critical.
This picture shows a typical fatigue fracture inside the transom on a boat powered by an outboard engine.
In this case, an attempt has been made to repair the crack but putty and gelcoat cannot mend structural damage.
Ideally, the boat should be repaired indoors to protect the work from rain and sun and to ensure a stable temperature. If working indoors is not possible, a tent should be made over the boat. All hardware and equipment which prevents access to the damaged area must be removed. A dust mask and eye and ear protection should be worn before any grinding starts. The grinding dust should be extracted at source. A commercial dust extractor or vacuum attached to the grinder can be used.
These schematic drawings illustrate the principle of laminate repair. The first two images show damage which has not penetrated the whole laminate. The next three show a two sided repair. Many books state that a scarf of 1:12 is sufficient for fibreglass repairs. This could be true for unloaded areas with thick laminates. However, for thinner laminates and loaded areas, the scarf should be at least 1:20. In many cases, a scarf of 1:40 or more must be used to ensure adequate adhesion and absorption of stresses in loaded areas.
A decision has to be taken on what kind of materials to use for laminating once the repair area has been identified and prepared. The following text is a guide to making this choice.
Prior to grinding, all surface contamination like oil and silicone should be washed off and removed with a suitable solvent. For grinding, 40 grit sandpaper is a good choice. In the example shown here, grinding has uncovered deep delaminations. To ensure a lasting repair, the full extent of the delaminated fibreglass must first be removed, no matter how far or deep it extends.
When the grinding is complete, the area to be laminated will likely be much bigger than suggested by the initial visual inspection.
For example, in this boat, tiny cracks in the gelcoat were visible on only one side of the engine well but grinding revealed that the delamination was just as deep on both sides.
Primary bonding occurs when two surfaces are connected directly to each other, forming a chemically homogenous laminate containing no weak bond line.
A fresh, or “green”, polyester laminate, has active molecules on the surface that will bind chemically to a new laminate. Laminating onto a green laminate gives a primary bond.
Apart from sanding off bumps and fibres which could cause defects and air pockets in the laminate, a fresh (green) polyester laminate requires no preparations before adding another layer.
How long the laminate surface remains active depends on a combination of the technical properties of the resin and the temperature during curing. Generally the open time for polyester resin is 24-48 hours.
When building a moderate sized boat, primary bonding can usually be achieved. When building large FRP boats, more time is needed to complete a layer of laminate and this makes operating within open time windows more difficult. Even so, achieving primary bonding between laminates in the main hull is crucial. In most cases, only secondary bonding will be achieved when laminating frames, stringers and bulkheads into larger boats.
An older polyester laminate is rarely completely cured. It will still have some reactive molecules that might, if properly sanded first, bond with the repair laminate. Wiping a sanded laminate lightly with styrene, immediately before applying a fresh polyester laminate, might also improve the bonding properties.
All repair work relies on secondary bonding. Consequently, stronger or additional replacement material will be needed to bring the damaged area back to its original strength.
When laminating over a cured laminate, the cross-linking reaction does not occur to a significant degree across the bond line. Since the polymer networks are discontinuous, the bond relies mainly on the adhesive strength of resin.
Choosing a resin for structural repair
In general, isophthalic polyester, vinylester, or epoxy resins are preferable to general purpose (GP) polyester resins for FRP repairs and alterations. After considering strength, cost and ease of processing for each, isophthalic polyester and vinylester resins are usually recommended for most repair work.
For more critical structural repairs, laminates made with epoxy resin are generally stronger (but not stiffer!). Epoxy resins are highly adhesive and have a longer shelf life
A SECONDARy BONDING TEST FOR RESINS
1. Prepare a small piece of the laminate to be repaired. 2. Apply 3 layers of reinforcement and resin.
3. Cure for one day.
4. Separate new laminates. This may require use of a chisel.
5. If the new laminate pulls fibres out of the old laminate, the bonding is good! 6. Another simple testing method is by using small dry wooden blocks as shown in
than polyester and vinylesters. These characteristics make epoxy ideal for emergency repair kits. As they require no solvents, epoxy resin does not contaminate the surface of the original laminate and shows no shrinkage when curing (less tension).
Epoxies do not hydrolyse and this together with good adhesion, low shrinkage and high ratio of elongation to break, makes them more liable to perform well as a primary bonded laminate. However, epoxies are intolerant of bad mix ratios and the setting time cannot be shortened or lengthened by altering the amount of hardener. In addition, an epoxy surface is definitely not active with styrene; therefore, any further rework on an epoxy boat or an epoxy repair will have to be made with epoxy.
A thorough cleaning and preparation of the bonding surface is very important to achieve good epoxy adhesion.
As part of the repair process, a secondary bonding test can be made as follows.
Choosing reinforcement for structural repair
If practical, the same reinforcement used when building the original boat should be used in the repair, especially if the part being repaired is heavily loaded and operating near its design limits. Use of lighter weight reinforcement will allow for better contact with the surface but the importance of this feature should be weighed against the importance of using the original reinforcement for maximum support.
Meanwhile, remember that there will be no continuous fibres attaching the old to the new laminate, and strength of the join will depend solely on adhesion of the new laminate to the old. Almost 100 percent of stiffness can be recovered if the laminate is
In this example, the resin chosen for use was epoxy, but vinylester might also have performed well. Bear in mind that this was a single-sided repair and the original polyester laminate was already showing weakness from fatigue.
The reinforcement was a mix of 290 g woven twill and 450 g Double Bias fibreglass, chosen because of its drape ability and good performance with epoxy. built up to its original thickness; however, the strength and fatigue properties of the repaired laminate will be weaker than the original. Dimension of the fibre bundles is critical for the repair to perform well because large bundles and heavy mats/fabrics obscure air and resin-rich pockets that are more likely to form at the borderline between the old and new laminates.
It is important to take all these matters into consideration when designing the repair laminate (see Figure 102). If additional reinforcement is required to maintain the boat’s overall strength, be careful to avoid excessive laminate build-up as this can increase the risk of developing stress concentrations.
It is important not to clean a freshly-sanded, porous, fibre laminate with acetone or solvent prior to lamination, unless it has been contaminated with oil or grease. If cleaning is necessary a light grinding with clean sandpaper after the washing is required followed by sufficient time to allow the solvent sufficient time to “air out” (evaporate). When solvent is absorbed by the porous surface, it “contaminates” the surface laminate and can dilute the new resin preventing optimum adhesion.
When using polyester, a light styrene wipe prior to laminating is the only acceptable procedure. A small amount of styrene will activate the surface slightly and improve adhesion. Too much styrene will weaken the bond line.
For repairs under the waterline, fresh styrene in the new polyester laminate is also liable to trigger hydrolysis (absorption of water) at an earlier stage than in the original laminate and cause premature failure in the borderline area between old and the new laminate.
An important issue when making repairs is to check the water content of the laminate with a moisture meter. If the laminate contains too much water, the bonding will fail sooner than it should and the new laminate will separate from the old one prematurely.
When it comes to the actual laminating, all the same procedures as for making a new boat must be followed including the maintainance of high quality control standard.
At this stage, the laminate build up has been completed and the surface has been ground flat to a nice “finish”. Use of any form of putty on structural repairs is to be carefully avoided. Putty has a short “elongation to break” ratio, and will break up and crack much faster than a laminate.
This picture shows the finished product. Topcoat has been applied, water sanded, buffed and polished to a decent gloss. Polyester topcoat can be used on top of epoxy as long as the epoxy is cured properly before the topcoat is applied. In this case, a 5 mm aluminum plate has also been attached to distribute pressure from the bolts over a larger area.
Cross-section showing structural damage to the frame of an FRP boat and the proper method of repair:
1. A fracture in the outer skin has penetrated the whole laminate, and caused delamination in the framework.
2. For the repair to be effective, the wooden frame must be cut and removed. Next, the hull laminate must be repaired as described earlier.
3. The frame has to be ground to a scarf wherever it will be joined with other laminate, and then bonded down with putty/glue and finished with a radius filet.
4. All lamination work on the frame is best done with easily drapable fabrics or 450 g/m² and lighter CSM.
1. This represents almost the same structural damage as shown in Figure 105, but viewed from the side.
2. The frame is shown cut and taken away making the damaged laminate accessable. In this case, no scarf in the core of the frame is required, as would be on a wooden boat, because this frame is filled with foam or air, which is not a structural member.
3. The place to cut and how to cut the frame will vary depending on the damage and will have to be estimated carefully in each case. Sometimes, when structural foam is involved, it is necessary to make a scarf in the same way as with a wooden frame. In some cases, “stepping” the scarf may also be an alternative. Using additional extra length reinforcement, such as unidirectional fibres along the top of the frame, must also be considered sometimes to add strength to the repair.
American Boat and Yacht Council and Structural Composites, Inc. No date. The Composite Boat Builder Certification (CBBC) compendium. (Web site: www.abycinc. org/).
American Composites Manufacturers Association (ACMA). 1995. Fundamentals of Polymer Resins for Composites Manufacturing. (Web site: www.acmastore.org/merchant. mvc?Screen=PROD&Product_Code=11-001-0&Category_Code=CB).
American Composites Manufacturers Association (ACMA). 2008a. CCT (Certified Composites Technician) Compendium. (Web site: www.acmanet.org).
American Composites Manufacturers Association (ACMA). 2008b. CM (Composites Manufacturing) Magazine. (Web site: www.acmanet.org/CM/index.cfm).
Anmarkrud, T. 2004. Composites repair compendium. NORBOAT/OS Boat.
Coackley, N.Fishing Boat Construction: 2. Building a fibreglass fishing boat. FAO Fisheries Technical Paper. No.321. Rome. FAO. 1991. 84p. (Available at ftp://ftp.fao.org/docrep/ fao/003/t0530e/t0530e00.pdf).
Composites Technology Magazine. 2008. (Web site: www.compositesworld.com).
Eric Green Associates. 1999. Marine composites. Second edition. Maryland, United States of America. ISBN 0-9673692-0-7 (Web site : www.marinecomposites.com - portions of this book can be down-loaded from this site).
FAO/ILO/IMO. 2005. Voluntary Guidelines for the Design, Construction and Equipment of Small Fishing Vessels.
Gerr, D. 1999. The elements of boat strength: for builders, designers and owners. McGraw-Hill.
Gulbrandsen, O. Fishing boat designs: 2. V-bottom boats of planked and plywood construction. FAO Fisheries Technical Paper, No. 134, Rev. 2. Rome, FAO. 2004. 64p. (Available at ftp://ftp.fao.org/docrep/fao/007/y5649e/y5649e00.pdf (English); ftp:// ftp.fao.org/docrep/fao/008/y5649f/y5649f00.pdf (French); ftp://ftp.fao.org/docrep/ fao/011/y5649p/ (Portuguese); and ftp://ftp.fao.org/docrep/fao/007/y5649s/y5649s00. pdf (Spanish))
Gulbrandsen, O. and Pajot, G. 1993. Safety guide for small offshore fishing boats. BOBP/ MAG/16. Madras. (Available at: ftp://ftp.fao.org/docrep/fao/field/006/ad533e/ad533e00. pdf).
IMO. 2007. IMO document SLF 51/5: Safety of Small Fishing Vessels – Consolidated text of the draft Safety recommendations for decked fishing vessels less than 12 metres in length and undecked fishing vessels.
Lacovara, R.R. 2001. American Composites Manufacturers Association. Certified composites technician compendium.
Neste Chemicals. 1992. Guide for mould construction.
Nicholson, I. 1985. Boat data book. Sheridan House, Inc. New York. ISBN 0-85177-345-1.
Nicholson, I. 1994. Surveying small craft. ISBN 0-924486-58-9.
Nordic Work Group. 1984. Nordic Boat Standards. Det Norske Veritas. Oslo. (Available at www.sigling.is/lisalib/getfile.aspx?itemid=2469 and www.sigling.is/lisalib/getfile. aspx?itemid=2468).
Professional BoatBuilder Magazine. (Web site: www.proboat.com). Reichhold/Norpol. No date. The little working guide.
Scott, R.J. 1996. Fibreglass boat design and construction. Second edition. The Society of Naval Architects and Marine Engineers. New Jersey, United States. 96-16973 CIP. Strong, A.B. 1996.Fundamentals of polymer resins for composites manufacturing. American
Composites Fabricators Association.
Structural Composites/Eric Green Associates. 2003. American Boat and Yacht Council,
Composite boat builder certification compendium.
Copying old boat designs for
construction with fibreglass
It is possible to use an old wooden boat as a plug by first drying out the wood and then covering it with fibreglass reinforced polyester (FRP). The rest of the process of building up the surface is the same
as described in the section Making the Plug.
It should be noted that not all old boats or canoes are of a suitable design to be copied directly in fibreglass. Wood and FRP have different mechanical properties. It is dangerous to think that, since FRP is stronger, it can easily be used to make the hull of any boat thinner and lighter.
If the design does not take into consideration the properties of FRP, the copied boat may loose stiffness quickly and be more exposed to fatigue.
The combination of an original wooden boat shape and the lighter weight of FRP could result in vessel instability and other less favourable seagoing characteristics.
This type of large traditional wooden canoe has demonstrated its seaworthiness and durability for generations, successfully going out to sea from shore through the surf, heavily loaded with nets.
This FRP boat was copied from a wooden canoe and was not old but already had broken frames and fatigue cracks in the bottom laminate.
The shape, size and use of these wooden boats make them unsuitable for exact reproduction as FRP copies. FRP is too brittle to survive such regular bending and the thinner walls make the structure vulnerable to fatigue.
The FRP version would have to be built much more heavily than this copy and with better designed and stronger stiffeners in order to withstand the stresses involved in carrying their typical load of fishing equipment and men out to sea through the heavy swell.
Covering old boats with FRP
Choosing to cover an old worn-out wooden boat with fibreglass reinforced polyester to keep it floating on the water is a big risk. Even if the old wood can be dried out completely, the likelyhood of keeping rot away for any reasonable length of time is not very good.
There is a good chance that, within a few years, rot will eat up the boat from the inside!
Adding two to three layers of FRP on the wood will seem to produce a stiff and dry boat, but after a few years problems will start. To be safe at sea for a longer time, a new boat should be built.
Wooden boat covered with FRP. 1. Fibreglass laminate is damaged/ hydrolysed by water
2. Open space exists between fibreglass and wood with no bonding between the layers.
3. Wood is rotten. FIGURE 109
Material list and hull lay-up for
HULL LAyUPFOR DECk AND BUOyANCy TANkS, SEE ALSO FIGURE 7
NO ITEM STRIP WIDTH mm LAyUP CSM g/m2 TOTAL g/m2 AREA m2 TOTAL CSM kg 1 Whole area 1 x 300 300 12.3 3.7 2 Keel reinforcement 300 2 x 450 900 1.0 0.9 3 Side keels 100 1 x 450 450 0.6 0.3 4 Transom corner 100 2 x 450 900 0.3 0.3 5 Stem 150 2 x 450 900 0.2 0.2 6 Bottom reinforcement 1 x 450 450 5.7 2.6 7 Sheer reinforcement 100 1 x 450 450 1.0 0.5 8 Whole area 3 x 450 + 1 x 300 1650 12.3 20.3
9 Strip over keel 150 3 x 450 1350 0.5 0.7
10 Strip over rubbing keel 150 3 x 450 1350 0.6 0.8 Total CSM 30.3 kg Additional 10% 3.0 kg Total CSM 33 kg
ITEM LAyUP CSM g/m2 AREA
1 Coaming 300 + 3 x 450 1650 3.07 5.06
2 Deck aft, engine well ” ” 1.09 1.80
3 Deck forward ” ” 0.95 1.57
4 Floatation boxes aft ” ” 1.00 1.65
5 Thwart boxes ” ” 1.20 1.98
6 Floatation forward ” ” 0.74 1.22
7 Floor forward ” ” 0.46 0.76
8 Strip in flange, assembly 450 450 0.40 0.18
CSM 14.22 kg
Waste 10 % 1.42
CSM Total 15.6 kg
Polyester, 30 % glass content: 2.40 x 15.6 37.4 kg Total deck and floatation: FRP materials 53 kg
Wood fender and thward 14
TOTAL 67 kg
COAMING, DECk AND FLOATATION BOXES TABLE 2
Polyester resin with glass content = 30% = 2.4 x 33 kg = 79 kg Total weight of FRP in hull = 112 kg Coaming, deck, floating boxes = 67 kg Total weight of boat = 179 kg
These are approximate figures of the total amount of material needed: Gelcoat: 20 kg Polyester: 150 kg MEK Peroxide: 4 kg 300 g/m2 CSM mat: 14 kg 450 g/m2 CSM mat: 50 kg Acetone: 10 kg
Mould release wax: 0.3 kg PVA release agent: 0.2 kg Buffing compound: 0.2 kg
PU foam: As required
Polystyrene foam: As required Hardware:
PVC or wooden fender
Reinforcement plate of steel or aluminium Two to four stainless steel U-bolts
Bolts and nuts for fastening
Total layup and thicknesses:
Bottom 2 x 300 + 4 x 450 = 2 400 g/m2 t = 5.6 mm Sides 2 x 300 + 3 x 450 = 1 950 g/m2 t = 4.6 mm Keel 2 x 300 + 6 x 450 = 3 300 g/m2 t = 7.7 mm Side keels 2 x 300 + 5 x 450 = 2 850 g/m2 t = 6.7 mm Sheer 2 x 300 + 4 x 450 = 2 400 g/m2 t = 5.6 mm Stem 2 x 300 + 6 x 450 = 3 300 g/m2 t = 7.7 mm
Offset table MDV-1½ width from centre line Keel underside 12 12 25 25 25 25 25 19 12 Rabbet 12 23 35 35 33 32 31 25 12 Sprayrail, inner 618 466 275 31 Sprayrail, outer 640 506 314 35 Sheer 669 762 817 843 838 801 722 587 367 WL 1 450 549 641 675 643 536 379 183 WL 1 A 553 640 710 746 718 611 438 228 WL 2 586 676 741 773 754 667 519 274 12 WL 3 625 718 777 802 790 717 576 360 64 WL 4 648 738 796 821 810 755 629 420 121 WL 5 661 754 811 836 826 782 677 486 188 WL 6 719 553 271 Height from baseline Keel underside 151 35 0 0 0 0 5 47 307 Rabbet 151 137 120 102 85 67 63 78 307 Sprayrail 251 267 290 316 353 Sheer 694 680 668 669 679 697 724 762 815 Buttock A 164 146 127 110 101 91 100 176 Buttock B 183 162 142 126 126 126 157 Buttock C 211 188 165 147 155 173 272 TABLE 3
Technical information on GP
9 7 8 9 2 5 1 0 6 3 9 3 4 I1108E/1/10.09/1350 ISBN 978-92-5-106393-4 ISSN 2070-7010
In many areas of the world, finding the type of timber needed to build a good quality wooden boat is becoming a problem. As a result, fibreglass reinforced plastic (FRP) is beginning to be used by many wooden boatbuilders. The information provided in this
manual relates specifically to the production of a 4.5 m open fishing boat called the MDV-1. It is a simple, easily-driven, seaworthy boat intended for both rowing and power
propulsion. Its general-purpose design is suitable for inshore waters around the world. A general basic knowledge in the use of FRP as a boatbuilding material is presented and
step by step construction of a 4.5 m open fishing boat using FRP is set out in detail. In addition, the booklet describes how to maintain an FRP boat and how to recognize fatigue problems. Some simple guidelines on how to repair minor damage to FRP are also included. It is assumed that people planning to build a boat already have a good, general understanding of basic hand tool use. This manual should give boatbuilders and
fishermen a better understanding of how FRP acts, how to recognize fatigue problems and more serious damage, and how to carry out needed maintenance and repair.